DOI: 10.17188/1715608
title: Materials Data on Li6MnV3(PO4)6 by Materials Project

description: Li6V3Mn(PO4)6 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are twelve inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded to six O2- atoms to form distorted LiO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Li–O bond distances ranging from 2.13–2.50 Å. In the second Li1+ site, Li1+ is bonded in a rectangular see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.89–2.35 Å. In the third Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.99–2.71 Å. In the fourth Li1+ site, Li1+ is bonded in a see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 2.04–2.16 Å. In the fifth Li1+ site, Li1+ is bonded in a distorted rectangular see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.90–2.45 Å. In the sixth Li1+ site, Li1+ is bonded in a distorted trigonal non-coplanar geometry to three O2- atoms. There are a spread of Li–O bond distances ranging from 1.91–2.03 Å. In the seventh Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Li–O bond distances ranging from 2.17–2.46 Å. In the eighth Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.96–2.63 Å. In the ninth Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 2.04–2.38 Å. In the tenth Li1+ site, Li1+ is bonded in a see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 2.03–2.20 Å. In the eleventh Li1+ site, Li1+ is bonded in a trigonal non-coplanar geometry to three O2- atoms. There are a spread of Li–O bond distances ranging from 1.87–2.01 Å. In the twelfth Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 2.01–2.34 Å. There are six inequivalent V+3.33+ sites. In the first V+3.33+ site, V+3.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of V–O bond distances ranging from 1.95–2.16 Å. In the second V+3.33+ site, V+3.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra, an edgeedge with one MnO6 octahedra, and edges with two VO6 octahedra. There are a spread of V–O bond distances ranging from 1.97–2.05 Å. In the third V+3.33+ site, V+3.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of V–O bond distances ranging from 1.94–2.11 Å. In the fourth V+3.33+ site, V+3.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of V–O bond distances ranging from 1.96–2.11 Å. In the fifth V+3.33+ site, V+3.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of V–O bond distances ranging from 1.97–2.16 Å. In the sixth V+3.33+ site, V+3.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra, an edgeedge with one MnO6 octahedra, and edges with two VO6 octahedra. There are a spread of V–O bond distances ranging from 1.94–2.02 Å. There are two inequivalent Mn2+ sites. In the first Mn2+ site, Mn2+ is bonded to six O2- atoms to form distorted MnO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of Mn–O bond distances ranging from 1.94–2.32 Å. In the second Mn2+ site, Mn2+ is bonded to six O2- atoms to form distorted MnO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of Mn–O bond distances ranging from 2.03–2.42 Å. There are twelve inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one LiO6 octahedra, corners with two VO6 octahedra, and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 39–56°. There are a spread of P–O bond distances ranging from 1.54–1.61 Å. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one LiO6 octahedra, corners with two VO6 octahedra, and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 38–57°. There are a spread of P–O bond distances ranging from 1.53–1.60 Å. In the third P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one LiO6 octahedra, a cornercorner with one MnO6 octahedra, and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 44–54°. There are a spread of P–O bond distances ranging from 1.52–1.59 Å. In the fourth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one LiO6 octahedra, a cornercorner with one MnO6 octahedra, and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 38–58°. There are a spread of P–O bond distances ranging from 1.53–1.60 Å. In the fifth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one LiO6 octahedra and corners with four VO6 octahedra. The corner-sharing octahedra tilt angles range from 38–58°. There are a spread of P–O bond distances ranging from 1.53–1.60 Å. In the sixth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one LiO6 octahedra, a cornercorner with one MnO6 octahedra, and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 38–54°. There are a spread of P–O bond distances ranging from 1.51–1.61 Å. In the seventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one LiO6 octahedra, a cornercorner with one MnO6 octahedra, and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 37–54°. There are a spread of P–O bond distances ranging from 1.53–1.60 Å. In the eighth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one LiO6 octahedra, a cornercorner with one MnO6 octahedra, and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 37–55°. There are a spread of P–O bond distances ranging from 1.53–1.61 Å. In the ninth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one LiO6 octahedra and corners with four VO6 octahedra. The corner-sharing octahedra tilt angles range from 36–54°. There are a spread of P–O bond distances ranging from 1.52–1.61 Å. In the tenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one LiO6 octahedra, a cornercorner with one MnO6 octahedra, and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 40–53°. There are a spread of P–O bond distances ranging from 1.51–1.61 Å. In the eleventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one LiO6 octahedra, a cornercorner with one MnO6 octahedra, and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 40–52°. There are a spread of P–O bond distances ranging from 1.54–1.58 Å. In the twelfth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one LiO6 octahedra, a cornercorner with one MnO6 octahedra, and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 37–54°. There are a spread of P–O bond distances ranging from 1.53–1.58 Å. There are forty-eight inequivalent O2- sites. In the first O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the second O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Mn2+, and one P5+ atom. In the third O2- site, O2- is bonded in a 2-coordinate geometry to one Mn2+ and one P5+ atom. In the fourth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Mn2+ and one P5+ atom. In the fifth O2- site, O2- is bonded in a distorted rectangular see-saw-like geometry to three Li1+ and one P5+ atom. In the sixth O2- site, O2- is bonded in a 3-coordinate geometry to two V+3.33+ and one P5+ atom. In the seventh O2- site, O2- is bonded in a distorted trigonal pyramidal geometry to three Li1+ and one P5+ atom. In the eighth O2- site, O2- is bonded in a 3-coordinate geometry to one V+3.33+, one Mn2+, and one P5+ atom. In the ninth O2- site, O2- is bonded in a 3-coordinate geometry to two V+3.33+ and one P5+ atom. In the tenth O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one V+3.33+ and one P5+ atom. In the eleventh O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the twelfth O2- site, O2- is bonded in a 4-coordinate geometry to three Li1+ and one P5+ atom. In the thirteenth O2- site, O2- is bonded in a 4-coordinate geometry to three Li1+ and one P5+ atom. In the fourteenth O2- site, O2- is bonded in a trigonal planar geometry to one Li1+, one V+3.33+, and one P5+ atom. In the fifteenth O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one Mn2+ and one P5+ atom. In the sixteenth O2- site, O2- is bonded in a 3-coordinate geometry to two V+3.33+ and one P5+ atom. In the seventeenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the eighteenth O2- site, O2- is bonded in a 2-coordinate geometry to two Li1+ and one P5+ atom. In the nineteenth O2- site, O2- is bonded in a 3-coordinate geometry to two V+3.33+ and one P5+ atom. In the twentieth O2- site, O2- is bonded in a 2-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the twenty-first O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+3.33+, and one P5+ atom. In the twenty-second O2- site, O2- is bonded in a 4-coordinate geometry to three Li1+ and one P5+ atom. In the twenty-third O2- site, O2- is bonded in a distorted trigonal planar geometry to one V+3.33+, one Mn2+, and one P5+ atom. In the twenty-fourth O2- site, O2- is bonded in a 2-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the twenty-fifth O2- site, O2- is bonded in a 4-coordinate geometry to three Li1+ and one P5+ atom. In the twenty-sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+3.33+ and one P5+ atom. In the twenty-seventh O2- site, O2- is bonded in a bent 150 degrees geometry to one V+3.33+ and one P5+ atom. In the twenty-eighth O2- site, O2- is bonded in a 3-coordinate geometry to two V+3.33+ and one P5+ atom. In the twenty-ninth O2- site, O2- is bonded in a 3-coordinate geometry to two V+3.33+ and one P5+ atom. In the thirtieth O2- site, O2- is bonded in a distorted trigonal pyramidal geometry to three Li1+ and one P5+ atom. In the thirty-first O2- site, O2- is bonded in a trigonal planar geometry to one Li1+, one V+3.33+, and one P5+ atom. In the thirty-second O2- site, O2- is bonded in a bent 150 degrees geometry to one V+3.33+ and one P5+ atom. In the thirty-third O2- site, O2- is bonded in a 3-coordinate geometry to two V+3.33+ and one P5+ atom. In the thirty-fourth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the thirty-fifth O2- site, O2- is bonded in a distorted trigonal planar geomet